Effect of isothermal bainitic transformation temperature...
Embed Size (px)
Transcript of Effect of isothermal bainitic transformation temperature...
© Copyright by International OCSCO World Press. All rights reserved. 2009 Research paper 169
2009 of Achievements in Materials and Manufacturing Engineering of Achievements in Materials and Manufacturing Engineering
Effect of isothermal bainitic transformation temperature on retained austenite fraction in C-Mn-Si-Al-Nb-Ti TRIP-type steel
A. Grajcar a,*, H. Krztoń b a Institute of Engineering Materials and Biomaterials, Silesian University of Technology, ul. Konarskiego 18a, 44-100 Gliwice, Poland b Institute for Ferrous Metallurgy, ul. K. Miarki 12, 44-100 Gliwice, Poland * Corresponding author: E-mail address: firstname.lastname@example.org
Received 11.03.2009; published in revised form 01.08.2009
Manufacturing and processing
AbstrAct Purpose: The aim of the paper is to determine the influence of isothermal bainitic transformation temperature on a fraction of retained austenite for a new-developed C-Mn-Si-Al-Nb-Ti TRIP-type steel. Design/methodology/approach: The thermo-mechanical processing was realized in a multi-stage compression test by the use of the Gleeble 3800 thermomechanical simulator. The steel was subjected to six variants of processing with an isothermal bainitic transformation temperature in a range from 250 to 500°C. Identification of phase composition was achieved using microstructure observations and X-ray diffraction. To determine the fraction of retained austenite the Rietveld method was applied. Findings: The maximum fraction of retained austenite equal up to 16% can be obtained for the temperatures of isothermal bainitic transformation from 400 to 450°C, while the maximum carbon content in the γ phase equal 1.5 wt.% is present at the temperature of 350°C. Below 350°C due to high Ms temperature, the largest grains of retained austenite located in the ferritic matrix transform to marteniste. In a temperature range from 350 to 450°C, the Msγ temperature has a negative value, stabilizing the retained austenite. Research limitations/implications: To determine in detail the influence of isothermal bainitic transformation conditions on a fraction of retained austenite, the knowledge of the effect of isothermal holding time is also important. Practical implications: The obtained microstructures and especially retained austenite fraction dependent on an isothermal bainitic transformation temperature can be useful in optimization of thermo-mechanical processing conditions of C-Mn-Si-Al TRIP-type steels. Originality/value: Combined colour etching and X-ray diffraction methods were applied for microstructure identification of modern group of TRIP steels predicted to use in the automotive industry. Keywords: Metallic alloys; TRIP steel; Thermo-mechanical processing; Compression test; Retained austenite Reference to this paper should be given in the following way: A. Grajcar, H. Krztoń, Effect of isothermal bainitic transformation temperature on retained austenite fraction in C-Mn-Si-Al-Nb-Ti TRIP-type steel, Journal of Achievements in Materials and Manufacturing Engineering 35/2 (2009) 169-176.
Journal of Achievements in Materials and Manufacturing Engineering
A. Grajcar, H. Krztoń
Volume 35 Issue 2 August 2009
Since the nineties of 20th century, automotive industry has reported high demands for steels connecting high strength and plastic properties as well as cold formability. A great contribution in development of new generation of steels was brought by international projects with participation of numerous steel industry companies which goal was to elaborate and produce components from high strength steels, using modern methods of forming and combining body parts and other assemblies of a vehicle [1-3]. Fulfilling the expectations of automotive industry was possible thanks to elaboration of the group of multiphase steels, consisting of soft ferritic matrix containing islands of martensite, bainite or bainitic-austenitic islands. Steels with such microstructure feature with characteristics of a composite material, perfectly combining high strength with required plasticity. They are steels with ferritic-martensitic microstructure DP-type (Dual Phase) [4, 5] and ferritic-bainitic with retained austenite TRIP-type (Transformation Induced Plasticity), undergoing hardening during technological forming of products as a result of martensitic transformation of phase [6-10].
These steels are characterized by ferritic-bainitic microstructure with retained austenite, which gradually transforming into martensite during pressing causes strong strain hardening, taking effect with a delay of sheet thinning, and in the conditions of tensile test – delay of neck initiation. It leads to obtaining high strength finished product and high plasticity, allowing application of high technological strains in a production process. These steels most often contain from 0.15 to 0.5%C, 1-2%Mn and up to 2%Si, which nowadays is completely or partially substituted by Al, introduced in the similar concentration [8, 11]. Such combination of chemical composition and proper heat treatment carried out after cold rolling of sheets, results in obtaining from 5 to 15% of retained austenite [6-8]. Heat treatment of TRIP steels consists in annealing of sheets in a range of temperatures between Ac1 and Ac3 with successive rapid cooling up to the isothermal bainitic transformation temperature in a range from 300 to 500°C [8, 11, 12]. Obtaining suitable fraction of retained austenite is possible due to the presence of Si or Al, effectively delaying precipitation of cementite during isothermal holding in a range of bainitic transformation.
The final mechanical properties depend upon kinetics of austenite into martensite transformation, which is strictly connected with phase stability, mostly dependent on carbon concentration in austenite [12-14], the size and arrangement of particles of this phase as well as its strength and the present state of stress [15, 16]. Thermodynamic stability of austenite is described by the temperature of martensitic transformation start Ms, expressed most often by a well known Andrews formula :
where: C, Mn, Ni, Cr, Mo – mass contents of the elements in the austenite.
Moreover, in the case of multiphase steels, taking into consideration silicon and aluminium is also very essential. The modification of Andrews equation regarding silicon was achieved by Li and others , while the effect of aluminium on retained
austenite was a subject of research performed by Mintz , who modified the dependence (1) into the following form:
Al30Si5.7 Mo5.7Cr1.12Ni7.17Mn4.30C423539Ms (2)
where: C, Mn, Ni, Cr, Mo, Si, Al – mass contents of the elements in the austenite.
On the basis of dependence (2), it can be observed that Si has a small influence on the Ms temperature, as distinct from Al, which has a destabilizing effect on retained austenite. Moreover, preservation of retained austenite in microstructure is favoured by increased concentration of Mn. Unfortunately, the effect of phase stabilization obtained by Mn is substantially weaker when comparing to carbon. For this reason, determination of changes of C concentration in phase according to the conditions of heat treatment has a fundamental significance for TRIP steels.
In the great number of cases, optimum plastic properties of multiphase steels are obtained in the conditions of heat treatment, being effective with the maximum fraction of retained austenite [20, 21]. However, Matsuda and others , basing on the research of 0.1C-1.6Mn-1.1Si steel, revealed that samples heat treated in the conditions assuring maximum participation of retained austenite are characterized with lower total and uniform elongation in comparison with samples consisting of 2% lower fraction of phase. It has a close connection with carbon concentration in retained austenite, which was equal 0.96% for the steel with lower participation of phase and 0.77% for the steel with maximum fraction of this phase. The result of understated concentration of carbon was a transformation of a part of austenite into martensite already during cooling from the temperature of heat treatment finish, and successively a rapid martensitic transformation in the initial stage of cold plastic deformation. In this regard, the most reliable parameter of mechanical stability of phase is considered in recent times to be a product of retained austenite fraction f and carbon concentration c in this phase [12, 23, 24].
There are several methods to determine the fraction of retained austenite, each of them has its own advantages and disadvantages. The most popular are: image analysis [9, 16], X-ray diffraction [12-14], neutron diffraction [21, 25], magnetic method [23, 26] and also the newest technique – EBSD . The application of X-ray diffraction to calculate the fraction of retained austenite gives the advantage over the other methods because the lattice constant of austenite can be calculated, giving at the same time the value of carbon content in austenite.
One of the fundamental solutions to retained austenite’s problem was formulated by Averbach – Cohen approach . According to this approach, the volume fraction of the austenite VA is calculated as following:
V R In/1